The curious case of exploding quantum dots: anomalous migration and growth behaviors of Ge under Si oxidation
© Wang et al.; licensee Springer. 2013
Received: 19 March 2013
Accepted: 14 April 2013
Published: 25 April 2013
We have previously demonstrated the unique migration behavior of Ge quantum dots (QDs) through Si3N4 layers during high-temperature oxidation. Penetration of these QDs into the underlying Si substrate however, leads to a completely different behavior: the Ge QDs ‘explode,’ regressing back almost to their origins as individual Ge nuclei as formed during the oxidation of the original nanopatterned SiGe structures used for their generation. A kinetics-based model is proposed to explain the anomalous migration behavior and morphology changes of the Ge QDs based on the Si flux generated during the oxidation of Si-containing layers.
Since their inception in the early 1980s , quantum dots (QDs) have found a widespread application in advanced electronics, photonics, memories, thermoelectrics, metrology, and biosensing devices [2–6]. For semiconductor QDs, the key challenge for the production of these mostly self-assembled nanostructures is to achieve precise control over the formation of QDs of desired sizes at specific locations and targeted depths of penetration within an embedding matrix. Our group has successfully demonstrated a unique approach to deliberately locate Ge QDs of desired sizes, locations, and depths within Si-based semiconductor nanostructures using the control available through lithographic nanopatterning and selective oxidation of the nanopatterned Si1-xGe x layers [7–10].
Given the remarkable, experimentally observed property of Ge QDs to ‘divine’ the presence of Si-bearing layers by preferentially migrating towards them, we decided to investigate this effect further by continuing the high-temperature oxidation process (Figure 1) to allow the spherical Ge QDs to ‘transit’ through the Si3N4 buffer layer and penetrate the pure Si substrate below (Figure 1c,d,e). However, when the Ge QD burrows through the Si3N4 buffer layer and encounters the Si substrate, a completely different phenomenon is observed (Figure 1f): the original spherical QD, instead of growing larger, ‘explodes’ into smaller Ge fragments that now appear to migrate away from the Si substrate with further oxidation. In a sense, this new behavior is parallel to the fantasy story, ‘The Curious Case of Benjamin Button,’  in which, with the passing of time, Button, rather than aging, instead regresses back to his early childhood. In a similar fashion, the large, spherical QDs appear to regress back to their origins as many smaller, irregularly shaped QDs originally generated within the as-oxidized Si1-xGe x layers.
The nominal QD fabrication process involves the tri-layer growth of 15- to 30-nm-thick Si3N4/20- to 60-nm-thick polycrystalline Si0.85Ge0.15/5-nm-thick SiO2 using low-pressure chemical vapor deposition over a Si substrate. The topmost, thin SiO2, layer is deposited as a hard mask for the subsequent plasma etching for producing the lithographically-patterned SiGe nanopillars. The SiO2 cap also prevents the evaporation of Ge during the final, high-temperature oxidation process for generating Ge QDs from the original SiGe layers. Using a combination of electron-beam lithography and SF6/C4F8 plasma patterning processes, SiGe nanopillar structures of various sizes (50- to 100-nm widths) were fabricated and then subjected to thermal oxidation at 900°C for 35 to 90 min in an H2O ambient for generating the Ge QDs. Oxidation times vary based on the thickness of the nanopillars. It takes between 5 and 25 min at 900°C within the H2O ambient to completely oxidize polycrystalline Si0.85Ge0.15 pillars that are between 20- and 60-nm thick and convert them into Ge crystallites.
CTEM, scanning transmission electron microscopy (STEM), and EDX were conducted using a JEOL JEM-2100 LaB6 transmission electron microscope (JEOL, Akishima-shi, Japan) and a FEI Tecnai Osiris transmission electron microscope (FEI, Hillsboro, OR, USA). Great care was taken to prepare clean TEM samples with no surface contamination. Additionally, STEM observations were conducted under conditions (200 KV and beam current of 100 μA) of minimal radiation-induced damage to the Ge QDs.
Results and discussion
Ge QDs in SiO2 matrix
The oxidation of each SiGe nanopillar proceeds radially inwards in an anisotropic manner and preferentially converts the Si within the pillar into SiO2, while squeezing the Ge released from solid solution within each poly SiGe grain into an irregular-shaped Ge crystallite that ostensibly assumes the crystal orientation and a portion of the morphology of the original poly SiGe grain (Figure 1b). Thus, within this newly formed SiO2 matrix, Ge nuclei, 5 to 7 nm in size, appear in a self-assembled cluster with random morphology and crystalline orientation. Further oxidation results in the observed Ostwald ripening behavior with some of the nuclei in proximity to the Si3N4 buffer layer growing at the expense of the other previously formed Ge nuclei. Additionally, as described previously, the Ostwald ripening and the overall change in morphology to a more spherical shape occur as a consequence of the Ge QD burrowing into the underlying Si3N4 buffer layer (Figure 1c,d,e).
Ge QDs in Si3N4 matrix
The Ge QD migrates through the underlying Si3N4 layer in a two-step catalytic process, during which the QD first enhances the local decomposition of the Si3N4 layer, releasing Si that subsequently migrates to the QD. In the second step, the Si rapidly diffuses through the QD, perhaps interstitially [16–20], and is ultimately oxidized at the distal surface of the QD, generating the SiO2 layer above the QD. It takes approximately 75 min for a 30-nm diameter Ge QD (Figure 1e) to transit through the 30-nm-thick Si3N4 layer and make contact with the Si substrate below.
Ge QDs encountering the Si substrate
Thus, we have shown that the Ge QD exhibits two distinct types of morphological and migrational behaviors depending on whether it encounters a Si3N4 layer or the Si substrate. As mentioned above, in a previous paper , we have provided a detailed explanation for the behavior of Ge QDs penetrating Si3N4 buffer layers. In this paper, we propose a new explanation for the radically different behavior of the very same QDs now interacting with the Si substrate. Here, we draw parallels from previous studies on the oxidation rate of silicon showing a marked dependence of the oxidation on the Ge content in Si and the oxygen flux [21–25].
SiGe ‘Shell’ formation: Upon ‘contact’ with the Si substrate, i.e., with a thin oxide separating the QD from the substrate, it becomes thermodynamically and kinetically favorable for Ge atoms to migrate from the QD and dissolve within the Si substrate to form a thin, cup-shaped SiGe alloy shell (Figure 2). This is because of the release of the free energy of mixing for the SiGe alloy [26, 27]. Assuming that the kinetics of Ge diffusion and alloying with Si is not rate-limiting at these high oxidation temperatures, we propose that the thickness (4 to 5 nm; observed from STEM and EDX images in Figure 2) and composition (40% to 60%; derived from the enhanced oxidation rate to be discussed below) of the SiGe shell is essentially determined by an equilibrium established between the lowering of free energy due to SiGe alloy formation while simultaneously accompanied by an increase in free energy due to the lattice strain experienced by the SiGe shell formed on the Si substrate . This thin SiGe shell formed on the Si substrate surface also plays a pivotal role in the very different behavior of the Ge QD during further oxidation. Unlike in the case of the Si3N4 oxidation, where no such SiGe surface layer exists, the SiGe shell is experimentally observed to significantly enhance the oxidation rate of the Si substrate by as much as 2 to 2.5 times. Figure 3a shows our experimental data for the oxidation kinetics of polycrystalline Si1-xGe x layers in an H2O ambient at 900°C. The enhancement in the oxidation rate of polycrystalline Si1-xGe x as a function of Ge composition appears to be well approximated by 1 + ax, where the enhancement factor a ranges from 2.5 to 3.05 and x is the mole fraction of Ge in a Si1-xGe x alloy. The enhancement factor for polycrystalline Si1-xGe x oxidation is very close to the previous results which report an enhancement factor of 2 to 4 for the oxidation of single crystalline Si1-xGe x layers over that for Si [21–23]. Using this relationship, we estimate the Ge content of our thin SiGe shell to be between 40% and 60%. In contrast to the Ge QD-enhanced oxidation of the Si3N4 buffer layers, where a nearly constant, approximately 2.5-nm thickness of SiO2 exists between the burrowing QD and the Si3N4 interface, the oxide thickness between the QD and the Si substrate (or between the SiGe shell and the bottom of the lowest Ge dew drop) appears to increase with time and follows the expected oxidation kinetics of SiGe layers (Figure 3b).
In the case of the Si3N4 oxidation, we proposed that the 2.5-nm oxide thickness separating the QD from the nitride was essentially determined by a dynamic equilibrium that exists between the concentration of Si atoms generated from the dissociation of the Si3N4 and the oxygen flux . The bulk of the Si atoms generated by the Si3N4 dissociation is consumed in generating SiO2 behind the Ge QD and thereby facilitating the burrowing process.
QD explosion: The higher Si atom fluxes appear to cause heterogeneous defect sites within the QD to now become ‘activated’ as new and additional sites for silicon oxidation. Proof for our proposed mechanism above can be derived, by analogy, from previous works on the dependence of Si oxidation on oxygen flux [25, 30]. It has been shown previously that the oxidation rate is indeed linearly dependent on oxygen flux, with the pre-factor term of the oxidation-kinetics equation being enhanced by the increased oxygen concentration. According to the Deal-Groove model , oxide thickness increases with oxidation time per the equation: x 0 2 + Ax 0 = B(t + τ), where τ corresponds to a shift in the time coordinate which corrects for the presence of the initial oxide layer. The parabolic rate constant B = 2D eff C */N 1 is proportional to the equilibrium concentration of the oxygen flux (C * ), which has been experimentally demonstrated to be proportional to the partial pressure of the oxidizing species in the gaseous ambient . D eff is the effective diffusion coefficient, and N 1 is the number of oxygen molecules incorporated per unit volume of the oxide layer. The coefficient A is independent of the partial pressure, leading to the linear rate constant B/A which linearly increases with oxygen flux as well.
In a similar manner, we propose that the higher Si fluxes being generated via substrate oxidation now make it possible for higher rates of oxidation to occur at heterogeneous defect sites including stacking faults and twins within the QD (Figure 1c,d) and hence cause it to ‘explode’ into multiple Ge fragments, almost identical in size to the as-oxidized Ge islands formed from the original SiGe nanopillars. With further silicon dioxide generation, the Ge ‘dew drops’ subsequently migrate outward, from the core of the original monolithic Ge QD from which they came with increasing time through the increase in the thickness of the SiO2 layers separating them. Eventually, Si atom diffusion from the substrate to the dew drops slows down as the oxide thickness between them and the substrate increases. This decreased supply of Si atoms results in the oxide layers between the dewdrops achieving a limiting thickness of 4 to 8 nm (Figure 3c).
We have observed the unique and anomalous phenomenon of completely different Ge QD growth and migration behaviors within Si3N4 layers versus within the Si substrate during high-temperature oxidation. The Ge migration behavior and morphology change appears to be directly dependent on the Si flux generated during the oxidation of Si-containing layers. When the flux of Si is low (as in the case of the Si3N4), the Ge migrates as a large, spherical QD that grows at the expense of smaller Ge nuclei. In contrast, when the Si flux is high, as in the oxidation of the Si substrate (enhanced by the formation of a thin SiGe shell), internal defect sites within the QD become activated as sites for Si oxidation, causing QD to explode and almost regress to its origins as smaller separated Ge nuclei.
This work was supported by the National Science Council of R. O. C. (NSC 101-3113-P-008-008 and NSC-99-2221-E-008-095-MY3).
- Ekimov AI, Onushchenko AA: Quantum size effect in three-dimensional microscopic semiconductor crystals. JETP Lett 1981, 34(6):345–349.Google Scholar
- Robledo L, Elzerman J, Jundt G, Atature M, Hogele A, Falt S, Imamoglu A: Conditional dynamics of interacting quantum dots. Science 2008, 320(5877):772–775. 10.1126/science.1155374View ArticleGoogle Scholar
- Astafiev O, Inomata K, Niskanen AO, Yamamoto T, Pashkin YA, Nakamura Y, Tsai JS: Single artificial-atom lasing. Nature 2007, 449(7162):588–590. 10.1038/nature06141View ArticleGoogle Scholar
- Tiwari S, Rana F, Chan K, Shi L, Hanafi H: Single charge and confinement effects in nano-crystal memories. Appl Phys Lett 1996, 69(9):1232–1234. 10.1063/1.117421View ArticleGoogle Scholar
- Harman T, Taylor P, Walsh M, La Forge B: Quantum dot superlattice thermoelectric materials and devices. Science 2002, 297(5590):2229–2232. 10.1126/science.1072886View ArticleGoogle Scholar
- Yang JM, Yang H, Lin LW: Quantum dot nano thermometers reveal heterogeneous local thermogenesis in living cells. ACS Nano 2011, 5(6):5067–5071. 10.1021/nn201142fView ArticleGoogle Scholar
- Chen KH, Chien CY, Li PW: Precise Ge quantum dot placement for quantum tunneling devices. Nanotechnology 2010, 21: 055302. 10.1088/0957-4484/21/5/055302View ArticleGoogle Scholar
- Chen KH, Chien CY, Lai WT, George T, Scherer A, Li PW: Controlled heterogeneous nucleation and growth of germanium quantum dots on nano-patterned silicon dioxide and silicon nitride substrates. J Crystal Growth & Design 2011, 11: 3222. 10.1021/cg200470fView ArticleGoogle Scholar
- Chien CY, Chang YJ, Chen KH, Lai WT, George T, Scherer A, Li PW: Nanoscale, catalytically-enhanced local oxidation of silicon-containing layers by ‘burrowing’ Ge quantum dots. Nanotechnology 2011, 22: 435602. 10.1088/0957-4484/22/43/435602View ArticleGoogle Scholar
- Kuo MH, Wang CC, Lai WT, George T, Li PW: Designer Ge quantum dots on Si: a heterostructure configuration with enhanced optoelectronic performance. Appl Phys Lett 2012, 101(11):223107.View ArticleGoogle Scholar
- Chang JE, Liao PH, Chien CY, Hsu JC, Hung MT, Lee SW, Chen WY, Hsu TM, George T, Li PW: Matrix and quantum confinement effects on optical and thermal properties of Ge quantum dots. J Phys D: Appl Phys 2012, 45(10):15303–15308.View ArticleGoogle Scholar
- Ostwald W: Lehrbuch der Allgemeinen Chemie, vol. 2, part 1. Leipzig: Engelmann; 1896.Google Scholar
- Ratke L, Voorhees PW: Growth and Coarsening: Ostwald Ripening in Material Processing. Heidelberg: Springer; 2002.View ArticleGoogle Scholar
- Stekolnikov A, Bechstedt F: Shape of free and constrained group-IV crystallites: influence of surface energies. Phys Rev B 2005, 72(12):125326.View ArticleGoogle Scholar
- “The Curious Case of Benjamin Button”. http://en.wikipedia.org/wiki/The_Curious_Case_of_Benjamin_Button_(film)
- Dunham ST, Plummer JD: Point‒defect generation during oxidation of silicon in dry oxygen.I. Theory. J Appl Phys 1986, 59(7):2541–2550. 10.1063/1.337003View ArticleGoogle Scholar
- Dunham ST: Interstitial kinetics near oxidizing silicon interfaces. J Electrochem Soc 1989, 136(1):250–254. 10.1149/1.2096596View ArticleGoogle Scholar
- Uematsu M, Kageshima H, Shiraishi K: Microscopic mechanism of thermal silicon oxide growth. Comput Mater Sci 2002, 24: 229–234. 10.1016/S0927-0256(02)00199-4View ArticleGoogle Scholar
- Leroy B: Stresses and silicon interstitials during the oxidation of a silicon substrate. Philosophical Magazine Part B 1987, 55(2):159–199. 10.1080/13642818708211202View ArticleGoogle Scholar
- Hu SM: Kinetics of interstitial supersaturation during oxidation of silicon. Appl Phys Lett 1983, 43(5):449–451. 10.1063/1.94384View ArticleGoogle Scholar
- Nayak DK, Kimjoo J, Park JS, Woo JCS, Wang KL: Wet oxidation of GeSi strained layers by rapid thermal processing. Appl Phys Lett 1990, 57(4):369–371. 10.1063/1.103694View ArticleGoogle Scholar
- LeGoues FK, Rosenberg R, Nguyen T, Himpsel F, Meyerson BS: Oxidation studies of SiGe. J Appl Phys 1989, 65(4):1724–1728. 10.1063/1.342945View ArticleGoogle Scholar
- Eugene J, LeGoues FK, Kesan VP, Iyer SS, d’Heurle FM: Diffusion versus oxidation rates in silicon‒germanium alloys. Appl Phys Lett 1991, 59(1):78–80. 10.1063/1.105528View ArticleGoogle Scholar
- Rabie MA, Haddara YM, Carette J: A kinetic model for the oxidation of silicon germanium alloys. J Appl Phys 2005, 98(7):074904. 10.1063/1.2060927View ArticleGoogle Scholar
- Deal BE, Grove AS: General relationship for the thermal oxidation of silicon. J Appl Phys 1965, 36(12):3770–3778. 10.1063/1.1713945View ArticleGoogle Scholar
- Brunner K: Si/Ge nanostructures. Rep Prog Phys 2002, 65: 27–72. 10.1088/0034-4885/65/1/202View ArticleGoogle Scholar
- Medeiors-Ribeiro G, Williams RS: Thermodynamics of coherently-strained GexSi1-x nanocrystals on Si(001): alloy composition and island formation. Nano Lett 2007, 7(2):223–235. 10.1021/nl062530kView ArticleGoogle Scholar
- Plummer JD, Deal MD, Griffin PB: Silicon VLSI Technology: Fundamentals, Practice and Modeling. New Jersey: Prentice Hall; 2000.Google Scholar
- Enomoto T, Ando R, Morita H: Thermal oxidation rate of a Si3N4film and its masking effect against oxidation of silicon. Jpn J Appl Phys 1978, 17: 1049–1058. 10.1143/JJAP.17.1049View ArticleGoogle Scholar
- Flint PS: The rates of oxidation of silicon. Los Angeles: Paper presented at the Spring Meeting of The Electrochemical Society, Abstract No. 94; 1962.Google Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.